International Journal of the Physical Sciences Vol. 6 (22), pp. 5153-5165, 2 October, 2011 Available online at http://www.academicjournals.org/IJPS DOI: 10.5897/IJPS11.705 ISSN 1992 - 1950 2011 Academic Journals
Full Length Research Paper
Finite element analysis (FEA) modeling on adhesive joint for composite fuselage model
F. Mustapha1, N. W. Sim1 and A. Shahrjerdi2*
1Department of Aerospace Engineering, Universiti Putra Malaysia, 43400 UPM Serdang, Selangor, Malaysia.
2Department of Mechanical Engineering, Malayer University, Iran.
Accepted 7 June, 2011
In this paper, a finite element modeling via ABAQUS/Explicit simulation on a novel fabrication miniature composite fuselage structure is presented. The fuselage structure is modeled as a continuum composite layup that consisted of a woven C-glass fiber/epoxy 200 g/m
2 composite laminated  with
the orthotropic elastic material properties and adhesively bonded butt joint. The adhesively bonded joint progression is modeled using cohesive elements technology. For the purpose of FEA modeling, an experiment of double cantilever beam (DCB) according to ASTM standard D5528 is performed to determine the adhesive mode-I critical toughness. The mode-I interlaminar fracture toughness data (GI) are calculated and compared by four different methods according to the ASTM standard: BT, beam theory, MBT, modified beam theory, CC, compliance calibration method and MCC, modified compliance calibration method. The results indicate that ABAQUS/Explicit is able to reproduce satisfactory adhesive joint behavior using cohesive elements and collapse modes under crushing process. Key words: Adhesively bonded joint, composite, fuselage structure, fracture toughness, finite element analysis (FEA).
INTRODUCTION Composite manufacturing process is a well-established branch of research in engineering materials and technology. For the past years, aircraft structures were made usually of aluminium, a material with great capacity for plastic deformation, hence, a natural capability to absorb energy in crash situations. In recent years, composite materials are employed more widely to construct aircraft structures such as control surfaces for aircraft parts. This research focuses on modeling of a novel fabrication technique of a miniature composite fuselage. One of the methods to fabricate fuselage structures is composite manufacturing process of filament winding. However, the disadvantages of this method can be formulated in terms of expensive equipment, long production times and lack of flexibility regarding the shape of the object to be wound (Koussios et al., 2004). Dahdi et al. (2009) have successfully developed a novel fabrication technique of a miniature composite fuselage. The objective of this novel fabrication is to evaluate the *Corresponding author. E-mail: email@example.com.
possibility of using combining mould technique to replace the technique of filament winding by integrating woven fiber composite laminated with adhesive butt joint to sustain axial compression impact from debonding failure. The success of the aforementioned novel fabrication technique encouraged the authors to further investigate the potential of this novel fabrication technique to implement in real aerospace world.
Based on Travesa (2006), computer simulations are referred as virtual mechanical testing to increase the reliability and to decrease the number of required tests to certify a composite structure. ABAQUS/Explicit was employed in this research as an FEA modeling software. The reliability of ABAQUS in the performance of the non-linear analysis on crushing analysis has been proved from the literatures. Furthermore, ABAQUS offer composite layups to facilitate the composite model set up and cohesive elements technology that allows user to define the material properties in modeling the progressive damage of adhesive bonded joint. There is reasonable amount of crushing simulation work done using ABAQUS. Bisagni (2005) studied the dynamic buckling due to impulsive loading of thin-walled carbon fiber
5154 Int. J. Phys. Sci.
Figure 1. Typical fracture mode of adhesive bonded joint
specimens (Sharifi and Choupani, 2008).
reinforced plastics (CFRP) shell structures under axial compression. The approach adopted is based on the equations of motion, which are numerically solved using a finite element code (ABAQUS/Explicit) and using numerical models validated by experimental static buckling tests. In recent studies by Tafreshi (2006, 2004), modeling of delaminated composite cylindrical shells under axial compression were considered and material was assumed to be linear. An experimental investigation into crushing behaviour of filamanent-wound laminated cone-cone intersection composite shell under uniform axial load and nonlinear finite element analysis using ABAQUS/Explicit on axially crushed cotton fibre composite corrugated tubes were presented (Mahdi et al., 2001, 2006). Tarfaoui et al. (2008) investigated both experimentally and numerically dynamic response and damage modeling of filament wound glass/epoxy tubes. Crush simulation and experimental validation on filament wound C-glass fiber/epoxy 200 g/m
2 miniature fuselage
have been carried out (Yidris and Mokhtar, 2007). In recent studies, the applicability of the cohesive element in predicting failure of adhesive joint has been presented in publications. Cohesive element was implemented for the simulation of delamination in fiber composites and crack propagation in adhesive joints (Fan et al., 2008). The model adopts a bilinear damage evolution law and uses critical energy release rate as the energy required for generating fully damaged unit area via ABAQUS/ Explicit through the user subroutine (VUMAT). The traction-separation law have been employed in the Wimmer et al. (2006) investigation. Interface elements and the traction-separation law described are available in ABAQUS. Damage mechanics of composite laminates was studied via cohesive element and ABAQUS can also be found in Seyed and Tamins (2009) research.
In this paper, an FEA model on composite cylindrical structures with adhesively bonded butt joint under axial
compression is proposed to investigate the structures strength and collapse modes. A DCB experimental test according to ASTM standard D5528 is first performed to determine the mode-I critical toughness of adhesive that is required to FEA modeling. It is noted that, the mechanical behavior of the adhesive, and hence, the modeling was designed to avoid extensive deformation of the adherends. Thus, material nonlinearities of intralaminar and interlaminar failure modes for a composite adherend are not taken into account in this research. These studies mainly addressed crushing load and collapse modes and debonding failure between adhesive and adherent on the miniature fuselage model. A progressive failure analysis on adhesive bonded joint has been demonstrated to simulate the damage initiation and evolution from initially uncracked surfaces until final failure in predicting the damage and mechanical strength. Composite element characteristics ABAQUS models a continuum shell composite layup using continuum shell elements that fully discretize an entire three-dimensional body. The thickness is determined from the element nodal geometry. Continuum shell elements have only displacement degrees of freedom. From a modeling point of view, continuum shell elements look like three-dimensional continuum solids, but their kinematic and constitutive behavior is similar to conventional shell elements and based on shell theory. Continuum shell composite layups are composed of plies made of different materials in different orientations. A layup can contain a different number of plies in different regions. Continuum shell composite layups are expected to have a single element through their thickness, and that single element contains multiple plies. The stacking direction of the continuum shell elements in the layup allows ABAQUS to model the through-thickness response more accurately. In addition, continuum shell composite layups take into account a double-sided contact and thickness change, which provides more accurate contact modeling than conventional shell composite layups. Hence, it is used in the proposed modeling.
Cohesive element Adhesive, cohesive and delamination are the three main failure types in adhesively bonded joints (Figure 1). Adhesive failure occurring is mainly due to interfacial cracking (debonding) at geometric boundaries due to stress concentrations caused by separation of adhesives from adherend. Well-bonded joints should fail within the adhesive layer (cohesive failure) or within the adherends (interlaminar failure/delamination) when broken (Sharifi and Choupani, 2008; Kang et al., 2005). The special features of this study are that the cracks are
Figure 2. The three modes of crack loading (Haugen, 1998).
Figure 3. DCB test specimen (Sim, 2010).
modelled by a special type of cohesive elements in the general-purposed finite element analysis package (ABAQUS, 2007). The cohesive elements, only available in ABAQUS version 6.5 or higher, are designed to model bonded interfaces (Yang et al., 2009). Cohesive elements are used to model crack initiation and propagation along a predefined interface. In ABAQUS, the constitutive response of cohesive elements may be based on a continuum description of the material or a traction-separation description of the interface. The continuum description is suitable when the actual thickness of the interface is being modeled. Alternatively, the traction-separation description is suitable when the thickness of the interface